1 Exploring float glass powder as corrosion resistant glass coating applied to concrete by flame spraying From the Faculty of Georesources and Materials Engineering of the RWTH Aachen University Submitted by Li, Zhang, M. Eng. from Huzhou, China in respect of the academic degree of Doctor of Engineering approved thesis Advisors: Univ.-Prof. Dr.rer. nat. Reinhard Conradt Univ.-Prof. Dr.-Ing. Michael Raupach Date of the oral examination: This thesis is available in electronic format on the university library s website
2 Acknowledgement First and foremost I would like to thank my supervisor Prof. Dr. rer. nat. Reinhard Conradt. I appreciate all his contributions of time, ideas, and opportunities to make my Ph.D. experiences productive. He taught me to not only grow as an engineer but also as an independent thinker. The spirit and enthusiasm he has for research is motivational for me during the Ph.D. pursuit and in my long-term career goals. All co-workers in the Institute of Mineral Engineering have provided me with immense help. I am especially grateful for Peter König, Petra Schott, and Coenen Ralf for their intensive support in my experiments. Additionally, the members in my group have been a source of friendships as well as good advice and collaboration. I very much appreciated Dr. Andreas Prange, Swantje Thiele, Katharina Philips, Vera Peters-Nießen, Simon Bartolomey, Kirsten Hellmann, Wolfgang Wilsmann, Lena Kalf, Tanja Mund who I have had pleasure to work with. Additionally, I am also thankful for Prof. Dr.-Ing. Michael Raupach and Till Büttner from the Institute of Building Materials Research for their valuable discussion, support, and collaboration. I would also like to thank for China Scholarship Council for giving me the funding for my Ph.D. pursuit in Germany. It provided me with unique opportunity to gain a wide breath of experience in a long run. Lastly, and most importantly, I would like to thank my parents. They raised me with full love and faithfully supported me in all my pursuit. Thank you.
3 Abstract Float glass was chosen as precursor material to generate protective coatings on concrete structures against chemical attack. The method of application was flame spraying. The feedstock for flame spraying was in form of powders. The preparation methods (dry ball milling and spray drying) affected the morphology, the particle size distribution and the spray ability of the coating powders. Compared to as-sprayed coatings from dry ball milled powders, coatings from the spray dried powders had a more favorable performance. No obvious open pores existed and a better adhesive performance was obtained. Influences of the process parameters (spraying distance and preheating) were evaluated based on the morphology of the as-sprayed coatings, indicating that a combination of 50 mm spraying distance and 500 C preheating led to a dense coating and sufficient adhesion. The tensile bonding strength and the corrosion resistance of the coatings were investigated. Failures in the tensile strength test occurred in the upper part of the concrete, indicating sufficient bonding strengths between the as-sprayed coatings and the substrates. In corrosion tests, the as-sprayed coating from a powder SD33, spray dried powder from a water-based suspension having 33 wt.% glass content, completely inhibited the penetration of the H 2 SO 4 solution going through the coating into the concrete. Furthermore, after 7 days of exposure to the acid solution, no corrosion phenomena were found in the samples, indicating the extraordinary corrosion resistance of this coating. Two mechanisms are responsible for pore formation in the flame sprayed glass coatings: Pores are formed from the entrapped gas. They are normally round and small, and the edges of those pores are smooth. Another mechanism is pore formation due to a lack of liquid from the molten deposits to fill the interstices between the overlapping splats; the interstitial pores are normally bigger (over 100 µm), and have an irregular or round shape with sharp edges. Porosity of the coatings is measured by image analysis, whereby an easy method has been developed to transfer the measured 2D images into 3D porosity. It is found that the coating from the powder SD33 possesses the lowest porosity.
4 Zusammenfassung Floatglas wurde als Ausgangsmaterial gewählt, um Schutzbeschichtungen gegen chemischen Angriff auf Beton zu erzeugen. Die Methode der Applikation war Flammspritzen. Als Ausgangsmaterial für das Flammspritzen dienten Glaspulver. Die Herstellungsverfahren des Pulvers (Trockenmahlung in der Kugelmühle und Nassmahlung mit anschließender Sprühtrocknung) beeinflussten die Morphologie, die Teilchengrößenverteilung und die Sprühfähigkeit der Pulver. Im Vergleich zu gespritzten Schichten aus trocken gemahlenem Pulver lieferten Beschichtungen aus dem sprühgetrockneten Pulver bessere Ergebnisse. Es existierten keine offensichtlichen offenen Poren und eine bessere Haftung wurde erzielt. Einflüsse der Prozessparameter (Sprühabstand und Vorwärmen) wurden aufgrund der Morphologie der gespritzten Beschichtungen analysiert. Es zeigte sich, dass eine Kombination von 50 mm Spritzabstand und 500 C Vorwärmung zu einer dichten Beschichtung und ausreichender Haftung führt. Die Haftzugfestigkeit und die Korrosionsbeständigkeit der Schichten wurden untersucht. Ausfälle im Zugversuch traten im oberen Teil des Betons auf, was auf eine ausreichende Haftung zwischen Beschichtungen und den Substraten schließen lässt. Korrosionstests haben gezeigt, dass die Beschichtung aus Pulver SD33, sprühgetrocknetes Pulver aus einer wässrigen Suspension mit 33 Gew.% Glasanteil, das Eindringen der H 2 SO 4 -Lösung durch die Beschichtung in den Beton vollständig hemmt. Außerdem wurden nach 7 Tagen Penetration mit saurer Lösung keine Korrosionserscheinungen in den Proben gefunden, was die außerordentliche Korrosionsbeständigkeit der Beschichtung verdeutlicht. Zwei Mechanismen sind verantwortlich für die Bildung von Poren in der flammgespritzten Glasbeschichtung: Zum einen werden die Poren aus dem eingeschlossenen Gas gebildet. Sie sind in der Regel rund und klein, und die Ränder dieser Poren sind glatt. Ein weiterer Mechanismus ist Porenbildung aufgrund des Fehlens von Flüssigkeit aus den bereits geschmolzenen Anteilen, um die Zwischenräume zwischen den überlappenden festen abgeflachten Partikel zu füllen; die interstitiellen Poren sind in der Regel größer (über 100 µm) und haben eine unregelmäßige oder runde Form mit scharfen Kanten. Die Porosität der Schichten
5 wurde mit Hilfe von Bildanalyse gemessen, wodurch eine einfache Methode entwickelt worden ist, um die gemessenen 2D-Bilder in 3D Porosität zu übertragen. Es konnte festgestellt werden, dass die Beschichtung aus dem Pulver SD33 die niedrigste Porosität aufweist.
6 Table of contents 1. Introduction and motivation Status of the art Protective coatings Status of protective coatings for concrete Application of glass coatings Coating technologies Comparing thermal spraying techniques Process parameters Particle morphology of coating powders Required properties of coatings Adhesion strength Structure and porosity Corrosion resistance Experiments Preparation and characterization of coating materials Substrate preparation Spraying process Spraying parameters Temperature measurement in the concrete during flame spraying Characterization of the coatings Morphology and phase analysis of the coatings Tensile bonding strength analysis Porosity measurement I
7 Corrosion resistance test Results Characterization of coating materials Composition and thermal expansion coefficient (α) Particle size distribution and morphology of the powders Temperature profile in the concrete during flame spraying Process parameters of flame-spraying Spraying distance Preheating temperature on the substrate surface Layer-substrate bonding Different glass powders as coating material Tensile bonding strength Anti-corrosion effect hours test days test Discussion Optimization of the powder preparation Mechanisms of pore formation and porosity measurement Influence of process parameters Conclusion Prospect References II
8 1. Introduction and motivation 1. Introduction and motivation Concrete is the most widely used construction material for sewer pipes applied in waste-water systems, in which the environment can be significant harsh resulting in a fast degradation of the concrete. In the worst situation, the degradation can be in the order of several millimeters per year. Deterioration of the concrete sewer may result in serious problems such as loss of ability to transport sewerage, contamination of the ground and even surface subsidence. Much research has been done about the mechanism of the chemical attack on the concrete in waste water systems. The most typical one is the concrete deterioration by biologically produced sulphuric acid 1, 2. Firstly, in the anaerobic condition of the wastewater, sulfate reducing bacteria convert sulfates (SO 2-4 ) into sulfides such as hydrogen sulphide (H 2 S) gas, and then in favorable conditions, the gas diffuses into the atmosphere above the water. Secondly, due to the alkalinity of the concrete, there is a relatively high ph moist layer around the concrete pipe above the waterline, and at this high ph level, the H 2 S gas is absorbed into the surface of the concrete and separated into HS- or S 2 -, which attracts more H 2 S into the moisture layer. In turn further H 2 S decomposes. The increase of H 2 S absorption decreases the ph of the concrete, which may make it become susceptible to attack. Thirdly, in the presence of oxygen above the water line, the concentrated H 2 S reacts with oxygen to form elemental sulphur. The thiocacillus bacteria oxidize the sulphur to form sulphuric acid (H 2 SO 4 ). Thus the biologically produced sulphuric acid is formed. It has been identified that this biologically produced H 2 SO 4 is the most typical corrosive agent in corroding the concrete in waste water systems. Next, H 2 SO 4 reacts with calcium hydroxide (Ca(OH) 2 ) in the concrete to form gypsum (CaSO 4 2H 2 O), eq Ca(OH) 2 + H 2 SO 4 CaSO 4 + 2H 2 O (CaSO 4 2H 2 O) 1.1 In the course of the attack, gypsum reacts with tricalcium aluminate (3CaO Al 2 O 3 ) to form ettringite ((CaO) 3 (Al 2 O 3 ) (CaSO 4 ) 3 32H 2 O), eq (CaSO 4 2H 2 O) + 3CaO Al 2 O H 2 O (CaO) 3 (Al 2 O 3 ) (CaSO 4 ) 32H 2 O 1.2 1
9 1. Introduction and motivation It is shown in Fig. 1.1 that the white substance above the water line is due to the formation of gypsum. The formations of gypsum and ettringite are expansive processes which lead to a cohesive loss of the cement matrix, and to possible expansion, cracking, spalling of the concrete. Fig Degradation formation (gypsum) on the concrete in the waste water system 2. Therefore, it is necessary to protect the inner site of the concrete pipes used in the wastewater systems from the harmful environment. Various organic coatings were already utilized on the concrete and evaluated according to their bonding and anticorrosion performance. Regarding the problems of organic coatings (high cost, durability problem, environmental pollution), glass could be a promising alternative coating material due to its low cost, chemical stability and environmental friendliness. Conventional technologies using a furnace cannot be applied to produce an onsite glass coating to the concrete pipes. Thermal spraying is a probable option due to its high flexibility in operational environment. It has been widely used to deposit glass or glass based composite coatings onto diverse substrates. Among different kinds of thermal spraying, flame spraying is commercially outstanding due to its simple equipment and low energy cost. However, there is hardly any studying about glass coating applied by flame spraying onto non-metallic substrate against chemical attack. In this work, the goal is to apply a glass coating with flame spraying onto the concrete surface against sulfuric acid corrosion. A commercial float glass has been chosen as the raw coating material instead of a specifically designed glass composition. 2
10 1. Introduction and motivation Besides, sodium silicate (water glass) is used as the bonding layer material. Flame spraying technology is applied here to produce the coating on the concrete, and the coating materials are in the form of powder. To analyze the correlation between the powder characteristics and the resulted coating, the preparation of the coating powders is divided into two ways: dry mechanical milling and wet milling with sequent spraydrying. The effect of process parameters, like preheating temperature, spraying distance, is investigated to optimize the as-sprayed glass coatings in terms of phase composition, morphology, bonding strength to the concrete substrate and capability of anti-corrosion. In chapter 2, the status of study in protective coatings, coating technologies, required properties of coatings is introduced. In chapter 3, the experimental procedure is presented. Results are listed in chapter 4, including characterization of the coating powders, characterization of the as-sprayed glass coatings produced with the different process parameters, effect of the bonding agent, comparison of the as-spraying coatings from the different coating powders, properties analysis consisting of the tensile bonding strength and the performance of corrosion resistance. Chapter 5 is the discussion composed of optimization of powder preparation, mechanisms of pore formation and porosity measurement, and influence of process parameters. Chapter 6 and 7 are the conclusion and prospect, respectively. 3
11 2. Status of the art 2. Status of the art 2.1. Protective coatings Status of protective coatings for concrete Application of protective coatings on concrete has received much attention. Most researches focused on utilizing an organic substance as coating material, such as rubber, epoxy, polyurethane, etc. Swamy et al. 3 applied a coating from acrylic rubber to protect the concrete structure from the aggressive environment. The result showed that this coating could prevent penetration of water, air, and chloride ions into the concrete. Delucchi et al. 4 pointed out that water permeability was a fundamental factor to evaluate the performance of protective coatings, because concrete is porous so that it is sensitive to a lot aggressive agents soluble in water. The authors compared the water permeability rates of four organic coatings on the concrete with two different methods. The first consisted in measuring the mass increase of the coated concrete brick as a function of time after exposure to the water; and the water permeability was calculated using the following equation 2.1: w 1 = m 1 S where w 1 (g/cm 2 h -0.5 ) was the water transmission rate, m 1 (g h -0.5 ) was the slope of the linear part of the plot of weight versus the square root of time, S 1 (21 cm 11 cm) was the area of the coated surface facing to the water. The second test was applied using a set-up as shown in Fig The water penetration into the Samples was monitored by recording the level of the water in the column (ø 6 mm). The water transmission rate was calculated according to the equation 2.2: w 2 = m 2 S c S s 2.2 4
12 2. Status of the art where w 2 (g/cm 2 per h 0.5 ) again was the water transmission rate, m 2 (mm/h 0.5 ) was the slope of the linear part of the plot of the column height versus the square root of time, S s (44 cm 2 ) was the area of the coated surface facing to the water; S c (28 mm 2 ) was the column cross-section. Results showed that rankings of the four coatings in terms of the water transmission rate were the same in both tests, but the small diameter of the column made the second test very sensitive to the effect of the water penetration, allowing to distinguish different coatings with only slight differences in the water permeability. Fig Testing apparatus for the evaluation of the water transmission rate of coatings in the studying by Delucchi et al. 4. Vipulanandan et al. 5 adopted a glass-fiber mat-reinforced epoxy coating onto the concrete structure. The lifetime of the coated concrete in 3% sulfuric acid could be extended by more than 70 times. Subsequently, the authors applied four commercially available epoxy-based coatings onto dry and wet concrete substrates, respectively. Two tests were used to compare the tensile bonding strength of the coatings to the concrete. The most promising result was that the epoxy coatings had a good bonding strength (>1.3 MPa) to both dry and wet concrete structures during 2 years of testing period 6. 5
13 2. Status of the art The study by Al-Zahrani et al. 7 compared protective coatings on steel-reinforced concretes based on their physical properties including water absorption, water permeability, chloride permeability and adhesion. In an accelerated corrosion test, a polyurethane based coating performed best, followed by a cement based polymermodified coating, an epoxy-based coating and a cement-based coating in descending order. Another study 8 compared the protecting performance of epoxy, polyurethane, acrylic, polymer, and chlorinated rubber coatings for the concrete in terms of water absorption, chemical resistance, chloride permeability and chloride diffusion. The results indicated that epoxy and polyurethane coatings were the best in decreasing the water absorption into the concrete, and the concrete substrates protected by these two coatings were also found relatively intact (only corners of the specimens damaged) after 60 days immersed in 2.5% sulfuric acid. The least coefficient of the chloride diffusion was measured in the concrete specimen coated with polyurethane followed by epoxy, acrylic and last rubber. In summary, researches of the organic protective coatings for the concrete substrates found that among various organic materials polyurethane and epoxy based coatings performed best against the chemical attack. However, it is unavoidable that the solvent-borne or water-borne organic coatings bring an environmental pollution because of volatile organic compounds (VOC) emission. A report 9 about concrete corrosion in the Hamburg sewer system said that the concrete pipes were destroyed to a depth > 6 cm within four to six years, although they had been coated with a thin layer of epoxy resin prior to application; up to 50% of the corroded concrete wall consisted of gypsum. This shows that the organic coatings have a durability problem. In addition, the high cost of the organic coatings limits large scale application. Therefore, it becomes senseful and challenging to find an alternative material for protective coatings on concrete Application of glass coatings Glass has been proposed as environmental barrier material for coatings on metallic or ceramic substrates. Significant works have been done on bioactive glass coatings to promote osteointegration and stability of titanium or titanium alloy implants. Schrooten et al. 10 produced an economical bioactive glass (BAG) coating from a 6
14 2. Status of the art composition (in wt.%): 52.0 SiO 2, 30.5 CaO, 9.8 Na 2 O, 6.2 P 2 O 5 and 1.5 CaF 2, for Ti6Al4V oral implant by plasma-spraying. The authors found that the adhesive strength of the resulting BAG coating was sufficient for a load-bearing oral application even after an in vitro reaction time of two months. In a study by Kim et al. 11, coatings of calcium and phosphate-based glasses (xcao-(0.55-x)na 2 O-0.45P 2 O 5 ) mixed with hydroxyapatite (HA) were applied on the ZrO 2 substrate by enameling technique. The effects of the glass composition (x=0.3, 0.4, 0.5 mol), of the ratio of glass to the HA, and of the enameling temperature on the coating properties were analyzed. It was found that a completely dense structure was obtained at high glass addition (50 wt.%), using a glass with a low CaO content (x=0.3 mol), and a heat treatment above 800 C for 2 h. Adhesion strengths of the composite coatings were much higher than those of pure HA coatings. Work by Peddi et al. 12 described a bioactive glass from the system Na 2 O-CaO- B 2 O 3, modified by additions of SiO 2, Al 2 O 3 and P 2 O 5. The authors produced a welladhered coating from this glass to titanium alloys by enameling. The resulting coating had an adhesive strength (36±2 MPa) and an excellent biocompatibility. Cannillo et al. 13 produced plasma-sprayed glass ceramic (apatite/wollastonite) coatings on titanium alloy substrates to increase their bioactivity after implantation into the body. The microstructure of the coatings possessed a lot of defects, such as pores and micro-cracks. A post-thermal treatment did not help to lower the porosity, but nevertheless was necessary to obtain crystalline phases in the glassy matrix to increase the mechanical properties of the coatings. Beyond the biomechanical field, glass and glass composite coatings have been used on other structures for coloring or for protection against high temperatures or corrosive environments. Tikkanen et al. 14 produced a glass coating on a glass surface by flame spraying for coloring decoration. It was found that the glass coating had a good adhesion on the glass substrate. The sintering of the sprayed glass particles could be improved by using small particle sizes of the powders, and a coating glass with a low viscosity at spray temperatures. A glass-alumina composite coating was produced employing waste glass as a low-cost raw material 15. The prepared glass powder, mixed with different percentages of alumina powder as reinforcement, was plasma sprayed on a stoneware substrate, and 7
15 2. Status of the art both as-sprayed and thermally post heated coatings were investigated for properties, including vickers microhardness, facture toughness and abrasion resistance. The authors pointed out that the as-sprayed glass coatings were too defective to be of technical interest: The glass particles did not completely flatten on the substrate. So a sufficient amount of reinforcing alumina had to be added, at least 40%. Besides, in another case from this researching group, glass-ceramic coatings were produced by plasma spraying to protect ceramic tile. A CaO-ZrO 2 -SiO 2 glass frit was the coating material 16. Its chemical resistance was not well controllable, since a crystallization forming wollastonite in the coating during the post-thermal treatment lowered its chemical resistance. However, sintering and crystallizing the as-sprayed coatings were key requirements in the thermal treatment: Only after crystallization, a significant increase in all mechanical properties (Vickers microhardness, elastic modulus, fracture toughness) could be obtained. In turn, the abrasion resistance of the protective coatings could exceed that of stoneware. Besides, the interface adhesion of the as-sprayed coating to the ceramic substrate already appeared to be good, and post-thermal treatment even enhanced it. This was not only because the mechanical interlocking was promoted by viscous flow, but also because crystals grew from the substrate interface into the coatings. In the group of Miranzo et al 17, a lot of works have been done to develop and investigate glass and glass-ceramic coatings via flame spraying. In one case, two refractory glass coatings from the compositions in the SiO 2 -Al 2 O 3 -Y 2 O 3 system, namely 66SiO 2-22Al 2 O 3-12Y 2 O 3 mol.% and 50SiO 2-30Al 2 O 3-20Y 2 O 3 mol.% (D), were in situ deposited on stainless steel substrates by flame spraying (oxy-acetylene flame). According to the phase diagram of the system SiO 2 -Al 2 O 3 -Y 2 O 3 (Fig. 2.2), one composition (G) was situated in the glass forming zone; another composition (D) was in a zone of glass formation with partial crystallization. In both coatings, the splat morphology was disc shaped, and the splat diameters were 50 µm and 36 µm for G and D coatings, respectively. The porosity quantification indicated that the D coating had only 2 vol.%, comparing with 13 vol.% for the G coating, and the mean pore size was 3.0 and 6.5 µm for G and D, respectively. Differences in the splat size and porosity between both coatings were related to the different glass transition temperatures and viscosities of the two compositions at spraying temperature. Glass G had a slightly lower viscosity. 8
16 2. Status of the art This supported spreading upon impact leading to the larger splat diameter, and also explained the higher number of bubbles observed in the G coating, since gases were more easily trapped. Besides, the higher the density of the bulk glass, the denser was the as-sprayed coating. Fig Glass formation region in the system SiO 2 -Al 2 O 3 -Y 2 O Glass-ceramic coating was also applied by conventional enameling technique as an oxidation resistance bond layer between a plasma-sprayed yttria stabilized zirconia (YSZ) top coating and a nickel based superalloy substrate 18. Functionally graded material (FGM) is characterized by gradual variation in composition and structure in space. It has been induced by application of the thermal sprayed glass coatings, since this is an efficient way to minimize the mismatch of the thermal expansion coefficient between coating material and substrate. For instance, glass-alumina graded coatings were produced via plasma spraying onto an alumina substrate 19. The glass belonged to the system CaO-ZrO 2 -SiO 2. Two different compositional gradients were developed: one reached from 100 vol.% alumina to 100 vol.% glass; another reached from vol.% glass to 100 vol.% glass. Results showed that it was only possible to sinter the glass, but not to crystallize it without delamination. However, when the coating already continued some glass at the very interface, it was possible to sinter and crystallize the glass phase to achieve enough mechanical properties. 9
17 2. Status of the art In a previous research at our institute 20, flame sprayed metal/glass coatings were applied onto a steel substrate (42CrMo4) to improve its chemical properties. Coating materials were powder mixtures of NiCr and lab-made glasses. Minimization of the α mismatch between the substrate and the coating material by varying the content of glass and metal in the mixture constituted the basis for choosing the coating material to insure a good adhesion of the coating to the substrate Coating technologies Coating technology is a discipline covering an extremely wide range. What we are discussing here is concerning thermal coating techniques only, mainly including conventional enameling technology using a furnace, sol-gel process with a consequent thermal treatment, and thermal spraying technology with various spraying guns. The conventional enameling process normally needs a relatively long time, and the applied temperature should be sustainable for the substrate so that its application to a concrete structure is not possible. Generally, the sol-gel process also needs a whole posttreatment and produces only a thin film (several micrometers). Thermal spraying is a general term to describe all methods in which the coating is formed from melted or semi-melted droplets. In the thermal spraying technology, the precursor material is usually used in the form of powder, wire or rod, which is fed into an electric arc or a flame produced by a spraying gun, where the formed droplets are accelerated towards the substrate. Thermal and kinetic energy of the flame flux can be produced either with combustible mixtures of fuel gas and oxygen, or by using an electrical power source. Based on the energy source, the thermal spraying technology mainly consists of plasma-spraying, combustion flame spraying, high-velocity flame spraying (HVOF) and electrical arc spraying Comparing thermal spraying techniques Many researches have compared these thermal spraying techniques, and mainly focused on the differences of their process parameters, such as velocity or flame temperature. In the work by Planche et al. 21, NiCrBSi powder was sprayed successively with plasma, flame and HVOF spraying, respectively. The characteristics of in-flight particles were monitored (see in Fig. 2.3), and the results indicated that the highest 10
18 2. Status of the art particle velocity was obtained for HVOF spraying, > 10 times superior to that obtained by flame spraying and about 3 times higher than that of plasma spraying. In contrast to the particle velocity, the lowest temperature of the impinging particles was found for HVOF, 500 K under the flame spraying and about 100 K below plasma spraying. The understanding of the difference between the methods is intended to serve researchers and manufacturers a valuable resource for choosing an appropriate thermal spraying technology for particular coating materials and substrates. Fig Particle temperature versus velocity for three different coating methods 21. Coating microstructures from the different spraying methods were also compared in this studying (Fig. 2.4). The coating obtained by flame spraying exhibited a structure having the thickest lamella and the largest pores. Using plasma spraying, most deposited particles flattened and the resulting coating also had a lamellar structure having a lower porosity than that of the flame sprayed coating. HVOF sprayed coating had a low porosity which could be probably related to the higher kinetic energy of the particles. 11